#------------------------------------------------------------------------------
#$Date: 2016-03-26 21:15:17 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180471 $
#$URL: svn://www.crystallography.net/cod/cif/7/21/40/7214042.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7214042
loop_
_publ_author_name
'Han, Bao-Xia'
'Wang, Chuan-Zeng'
'Chen, Kai'
'Xiao, Xin'
'Tao, Zhu'
'Xue, Sai-Feng'
'Zhang, Yun-Qian'
'Zhu, Qian-Jiang'
_publ_section_title
;
 Coordination and supramolecular assemblies of K+/Ln3+ to
 perhydroxycucurbit[5]uril in the presence of [PMo12O40]3−:
 potential application in isolation of light lanthanides
;
_journal_issue                   9
_journal_name_full               CrystEngComm
_journal_page_first              1615
_journal_paper_doi               10.1039/c3ce42063a
_journal_volume                  16
_journal_year                    2014
_chemical_formula_moiety
'C30 H34 N21 O25 K2, P Mo12 O40, 2(H3 O), 11(H2 O)'
_chemical_formula_sum            'C30 H62 K2 Mo12 N21 O78 P'
_chemical_formula_weight         3225.46
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 99.185(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   16.4852(11)
_cell_length_b                   14.4496(9)
_cell_length_c                   33.998(2)
_cell_measurement_temperature    223(2)
_cell_volume                     7994.6(9)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      223(2)
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'Bruker Smart Apex2 CCD Detector'
_diffrn_measurement_method       'φ and ω scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0583
_diffrn_reflns_av_sigmaI/netI    0.0498
_diffrn_reflns_limit_h_max       19
_diffrn_reflns_limit_h_min       -19
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       40
_diffrn_reflns_limit_l_min       -40
_diffrn_reflns_number            33378
_diffrn_reflns_theta_full        25.20
_diffrn_reflns_theta_max         25.20
_diffrn_reflns_theta_min         1.21
_exptl_absorpt_coefficient_mu    2.093
_exptl_absorpt_correction_T_max  0.6676
_exptl_absorpt_correction_T_min  0.6121
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Bruker, 2008)'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    2.680
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             6280
_exptl_crystal_size_max          0.26
_exptl_crystal_size_mid          0.23
_exptl_crystal_size_min          0.21
_platon_squeeze_details
;
;
_refine_diff_density_max         2.029
_refine_diff_density_min         -1.771
_refine_diff_density_rms         0.181
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.051
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     607
_refine_ls_number_reflns         7159
_refine_ls_number_restraints     11
_refine_ls_restrained_S_all      3.108
_refine_ls_R_factor_all          0.0719
_refine_ls_R_factor_gt           0.0608
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0462P)²+255.9086P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1457
_refine_ls_wR_factor_ref         0.1516
_reflns_number_gt                5884
_reflns_number_total             7159
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c3ce42063a.txt
_cod_data_source_block           p9
_cod_original_sg_symbol_H-M      'C 2/c'
_cod_database_code               7214042
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
O1W O 0.305(3) 1.434(3) -0.298(2) 0.22(3) Uani 1 1 d .
O2W O 0.256(5) 1.073(4) -0.159(3) 0.27(4) Uani 1 1 d .
O3W O -0.086(11) 1.930(11) -0.208(4) 0.28(9) Uani 0.50 1 d P
N11 N 0.0000 1.437(3) -0.2500 0.063(11) Uani 1 2 d SDU
O33 O -0.0636(17) 1.484(3) -0.244(2) 0.24(3) Uani 1 1 d D
O34 O 0.0000 1.351(3) -0.2500 0.27(4) Uani 1 2 d SDU
K1 K 0.1754(4) 1.4388(4) -0.28369(18) 0.0349(14) Uani 1 1 d .
O11 O 0.279(2) 0.8267(17) 0.0244(8) 0.086(5) Uani 1 1 d .
O12 O 0.0398(14) 0.8222(18) 0.0782(7) 0.060(7) Uani 1 1 d .
O13 O 0.222(2) 0.9991(17) 0.0066(8) 0.086(5) Uani 1 1 d .
O14 O 0.2662(14) 1.1595(17) -0.0295(7) 0.056(6) Uani 1 1 d .
O15 O -0.0390(15) 0.756(2) -0.0267(7) 0.076(9) Uani 1 1 d .
O16 O 0.151(2) 1.0395(17) -0.0658(8) 0.086(5) Uani 1 1 d .
O17 O 0.1113(15) 0.7814(19) 0.0172(7) 0.066(8) Uani 1 1 d .
O18 O -0.1030(14) 0.798(2) 0.0368(6) 0.071(8) Uani 1 1 d .
O19 O 0.009(2) 0.6515(15) 0.0390(7) 0.071(8) Uani 1 1 d .
O20 O 0.1324(14) 0.8968(16) -0.1220(6) 0.048(5) Uani 1 1 d .
O21 O 0.1318(15) 0.9022(18) 0.1432(6) 0.061(7) Uani 1 1 d .
O22 O 0.0066(15) 0.8432(17) -0.0855(11) 0.086(11) Uani 1 1 d .
O23 O 0.158(2) 0.8682(17) -0.0414(8) 0.086(5) Uani 1 1 d .
O24 O -0.1451(14) 0.7544(15) -0.0993(7) 0.054(6) Uani 1 1 d .
O25 O -0.1755(14) 0.851(2) -0.0342(6) 0.065(8) Uani 1 1 d .
O26 O 0.1754(14) 0.9081(19) 0.0680(7) 0.066(8) Uani 1 1 d .
O27 O -0.1284(16) 0.9422(16) -0.0966(11) 0.083(10) Uani 1 1 d .
O28 O -0.0098(17) 0.9825(16) 0.1086(11) 0.085(10) Uani 1 1 d .
O29 O 0.087(2) 0.986(2) -0.0151(11) 0.031(8) Uani 0.50 1 d P
O30 O -0.044(2) 0.907(2) -0.0034(10) 0.024(7) Uani 0.50 1 d P
O31 O 0.044(2) 0.927(2) 0.0246(10) 0.028(8) Uani 0.50 1 d P
O32 O 0.022(2) 1.029(2) 0.0444(9) 0.025(7) Uani 0.50 1 d P
P1 P 0.0000 1.0000 0.0000 0.026(2) Uani 1 2 d S
Mo1 Mo 0.00672(15) 0.76176(16) 0.02553(7) 0.0319(6) Uani 1 1 d .
Mo2 Mo -0.10342(15) 0.83532(17) -0.06800(8) 0.0349(6) Uani 1 1 d .
Mo3 Mo 0.19158(16) 0.88285(18) 0.01631(8) 0.0379(7) Uani 1 1 d .
Mo4 Mo 0.08661(15) 0.93004(17) 0.09810(7) 0.0320(6) Uani 1 1 d .
Mo5 Mo 0.17945(17) 1.11292(19) -0.02202(8) 0.0426(7) Uani 1 1 d .
Mo6 Mo 0.09066(19) 0.92496(18) -0.08265(8) 0.0419(7) Uani 1 1 d .
C1 C 0.1010(16) 1.6672(19) -0.2715(9) 0.032(6) Uani 1 1 d .
C2 C 0.0248(16) 1.7413(18) -0.2281(8) 0.030(6) Uani 1 1 d .
C3 C 0.1686(16) 1.678(2) -0.2013(9) 0.035(6) Uani 1 1 d .
H3A H 0.1720 1.7299 -0.1828 0.042 Uiso 1 1 calc R
H3B H 0.2190 1.6772 -0.2132 0.042 Uiso 1 1 calc R
C4 C -0.0096(16) 1.6773(19) -0.1631(8) 0.032(6) Uani 1 1 d .
H4A H -0.0607 1.6759 -0.1519 0.038 Uiso 1 1 calc R
H4B H 0.0239 1.7285 -0.1505 0.038 Uiso 1 1 calc R
C5 C 0.2004(17) 1.511(2) -0.1878(8) 0.035(6) Uani 1 1 d .
C6 C 0.1244(16) 1.585(2) -0.1450(8) 0.034(6) Uani 1 1 d .
C7 C 0.1378(15) 1.480(2) -0.1322(8) 0.034(6) Uani 1 1 d .
C8 C -0.0029(16) 1.511(2) -0.1474(8) 0.034(6) Uani 1 1 d .
C9 C 0.2153(16) 1.352(2) -0.1604(8) 0.037(7) Uani 1 1 d .
H9A H 0.2295 1.3322 -0.1326 0.044 Uiso 1 1 calc R
H9B H 0.2658 1.3511 -0.1721 0.044 Uiso 1 1 calc R
C10 C 0.0359(17) 1.353(2) -0.1236(8) 0.035(6) Uani 1 1 d .
H10A H 0.0778 1.3338 -0.1012 0.042 Uiso 1 1 calc R
H10B H -0.0170 1.3548 -0.1139 0.042 Uiso 1 1 calc R
C11 C 0.1613(17) 1.260(2) -0.2199(9) 0.035(6) Uani 1 1 d .
C12 C 0.1008(17) 1.232(2) -0.1630(8) 0.036(7) Uani 1 1 d .
C13 C 0.0600(17) 1.1661(19) -0.1976(9) 0.037(7) Uani 1 1 d .
C14 C -0.0406(18) 1.260(2) -0.1786(9) 0.037(7) Uani 1 1 d .
C15 C 0.0898(17) 1.1475(19) -0.2689(9) 0.037(7) Uani 1 1 d .
H15A H 0.1405 1.1489 -0.2806 0.045 Uiso 1 1 calc R
H15B H 0.0745 1.0825 -0.2663 0.045 Uiso 1 1 calc R
N1 N 0.0989(13) 1.6913(16) -0.2326(7) 0.032(5) Uani 1 1 d .
N2 N 0.1649(13) 1.5920(16) -0.1788(7) 0.033(5) Uani 1 1 d .
N3 N -0.0289(13) 1.6942(15) -0.2056(7) 0.028(5) Uani 1 1 d .
N4 N 0.0342(13) 1.5912(15) -0.1539(7) 0.030(5) Uani 1 1 d .
N5 N 0.1850(14) 1.4461(17) -0.1611(7) 0.036(5) Uani 1 1 d .
N6 N 0.1584(14) 1.2852(16) -0.1813(7) 0.034(5) Uani 1 1 d .
N7 N 0.0553(14) 1.4448(16) -0.1358(7) 0.036(5) Uani 1 1 d .
N8 N 0.0314(14) 1.2840(16) -0.1544(7) 0.034(5) Uani 1 1 d .
N9 N 0.1056(14) 1.1892(16) -0.2296(7) 0.034(5) Uani 1 1 d .
N10 N -0.0252(14) 1.1937(16) -0.2042(7) 0.036(5) Uani 1 1 d .
O1 O 0.1567(12) 1.6275(15) -0.2838(6) 0.042(5) Uani 1 1 d .
O2 O 0.2413(12) 1.4989(14) -0.2139(6) 0.040(5) Uani 1 1 d .
O3 O 0.2056(12) 1.2907(15) -0.2413(6) 0.041(5) Uani 1 1 d .
O4 O -0.0775(11) 1.4981(15) -0.1506(7) 0.046(5) Uani 1 1 d .
O5 O -0.1084(12) 1.2935(15) -0.1764(6) 0.043(5) Uani 1 1 d .
O6 O 0.0474(12) 1.8277(13) -0.2126(6) 0.038(5) Uani 1 1 d .
H6 H 0.0057 1.8600 -0.2127 0.056 Uiso 1 1 calc R
O7 O 0.1538(12) 1.6495(16) -0.1163(6) 0.048(5) Uani 1 1 d .
H7 H 0.2036 1.6405 -0.1087 0.072 Uiso 1 1 calc R
O8 O 0.1783(12) 1.4662(16) -0.0936(6) 0.044(5) Uani 1 1 d .
H8 H 0.2224 1.4951 -0.0903 0.066 Uiso 1 1 calc R
O9 O 0.1389(14) 1.1893(16) -0.1285(6) 0.050(6) Uani 1 1 d .
H9 H 0.1749 1.1536 -0.1339 0.075 Uiso 1 1 calc R
O10 O 0.0679(14) 1.0734(14) -0.1891(7) 0.048(5) Uani 1 1 d .
H10 H 0.0414 1.0604 -0.1711 0.073 Uiso 1 1 calc R
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O34 N11 O33 121.9(13) . .
O34 N11 O33 121.9(13) . 2_554
O33 N11 O33 116(3) . 2_554
O34 N11 K1 90.4(7) . 2_554
O33 N11 K1 32.9(17) . 2_554
O33 N11 K1 146.3(18) 2_554 2_554
O34 N11 K1 90.4(7) . .
O33 N11 K1 146.3(18) . .
O33 N11 K1 32.9(17) 2_554 .
K1 N11 K1 179.2(13) 2_554 .
N11 O33 K1 129(2) . 2_554
O1W K1 O33 160(2) . 2_554
O1W K1 O3 89.4(18) . .
O33 K1 O3 95.9(14) 2_554 .
O1W K1 O2 86(2) . .
O33 K1 O2 76.8(17) 2_554 .
O3 K1 O2 75.7(7) . .
O1W K1 O5 101.5(15) . 2_554
O33 K1 O5 98.2(13) 2_554 2_554
O3 K1 O5 69.9(7) . 2_554
O2 K1 O5 144.5(7) . 2_554
O1W K1 O4 107(2) . 2_554
O33 K1 O4 80.6(18) 2_554 2_554
O3 K1 O4 140.1(7) . 2_554
O2 K1 O4 139.7(7) . 2_554
O5 K1 O4 71.3(7) 2_554 2_554
O1W K1 O1 98.0(14) . .
O33 K1 O1 67.6(11) 2_554 .
O3 K1 O1 146.6(7) . .
O2 K1 O1 72.5(6) . .
O5 K1 O1 138.7(7) 2_554 .
O4 K1 O1 68.2(6) 2_554 .
O1W K1 O2W 55(2) . 4_554
O33 K1 O2W 118.6(18) 2_554 4_554
O3 K1 O2W 144.6(16) . 4_554
O2 K1 O2W 103.0(14) . 4_554
O5 K1 O2W 109.8(13) 2_554 4_554
O4 K1 O2W 60.3(17) 2_554 4_554
O1 K1 O2W 55.1(12) . 4_554
O1W K1 N11 172(2) . .
O33 K1 N11 17.8(6) 2_554 .
O3 K1 N11 84.3(7) . .
O2 K1 N11 86.9(5) . .
O5 K1 N11 81.6(7) 2_554 .
O4 K1 N11 81.1(5) 2_554 .
O1 K1 N11 84.4(8) . .
O2W K1 N11 131.1(16) 4_554 .
O1W K1 C5 104(2) . .
O33 K1 C5 59.8(18) 2_554 .
O3 K1 C5 74.5(7) . .
O2 K1 C5 17.8(6) . .
O5 K1 C5 135.6(7) 2_554 .
O4 K1 C5 132.0(7) 2_554 .
O1 K1 C5 72.1(7) . .
O2W K1 C5 114.6(13) 4_554 .
N11 K1 C5 69.1(5) . .
O1W K1 C11 106.0(19) . .
O33 K1 C11 79.3(13) 2_554 .
O3 K1 C11 16.8(6) . .
O2 K1 C11 74.6(7) . .
O5 K1 C11 70.0(7) 2_554 .
O4 K1 C11 132.8(7) 2_554 .
O1 K1 C11 137.4(7) . .
O2W K1 C11 161.4(16) 4_554 .
N11 K1 C11 67.6(7) . .
C5 K1 C11 68.3(7) . .
O1W K1 C14 117.7(15) . 2_554
O33 K1 C14 81.9(13) 2_554 2_554
O3 K1 C14 69.4(7) . 2_554
O2 K1 C14 136.7(7) . 2_554
O5 K1 C14 16.4(6) 2_554 2_554
O4 K1 C14 70.7(7) 2_554 2_554
O1 K1 C14 131.8(7) . 2_554
O2W K1 C14 120.3(14) 4_554 2_554
N11 K1 C14 65.2(7) . 2_554
C5 K1 C14 123.3(7) . 2_554
C11 K1 C14 64.5(7) . 2_554
Mo4 O12 Mo1 138.6(15) . .
Mo3 O13 Mo5 141.2(19) . .
Mo1 O15 Mo2 139.1(18) . .
Mo5 O16 Mo6 140.8(18) . .
Mo1 O17 Mo3 140.7(16) . .
Mo5 O18 Mo1 138.4(16) 5_575 .
Mo6 O22 Mo2 138.0(17) . .
Mo6 O23 Mo3 139.2(18) . .
Mo2 O25 Mo5 140.7(13) . 5_575
Mo3 O26 Mo4 140.0(14) . .
Mo2 O27 Mo4 138.7(19) . 5_575
Mo4 O28 Mo6 136.6(17) . 5_575
P1 O29 Mo3 124(2) . .
P1 O29 Mo5 122.6(18) . .
Mo3 O29 Mo5 95.3(12) . .
P1 O29 Mo6 120.0(17) . .
Mo3 O29 Mo6 94.1(12) . .
Mo5 O29 Mo6 93.9(13) . .
P1 O30 O31 55.5(16) . .
P1 O30 O32 56.0(15) . 5_575
O31 O30 O32 95(2) . 5_575
P1 O30 Mo1 127.6(18) . .
O31 O30 Mo1 72.3(17) . .
O32 O30 Mo1 133(2) 5_575 .
P1 O30 Mo2 123.5(18) . .
O31 O30 Mo2 141(2) . .
O32 O30 Mo2 67.7(15) 5_575 .
Mo1 O30 Mo2 93.4(11) . .
P1 O31 O30 58.5(17) . .
P1 O31 O32 58.4(16) . .
O30 O31 O32 99(2) . .
P1 O31 Mo1 127.1(19) . .
O30 O31 Mo1 68.7(16) . .
O32 O31 Mo1 140(2) . .
P1 O31 Mo4 126.3(19) . .
O30 O31 Mo4 132(2) . .
O32 O31 Mo4 68.0(15) . .
Mo1 O31 Mo4 92.1(11) . .
P1 O32 O31 53.7(15) . .
P1 O32 O30 54.2(15) . 5_575
O31 O32 O30 93(2) . 5_575
P1 O32 Mo4 125.4(18) . .
O31 O32 Mo4 71.8(16) . .
O30 O32 Mo4 142(2) 5_575 .
P1 O32 Mo2 124.5(18) . 5_575
O31 O32 Mo2 134(2) . 5_575
O30 O32 Mo2 70.5(15) 5_575 5_575
Mo4 O32 Mo2 94.2(11) . 5_575
P1 O32 Mo6 119.7(17) . 5_575
O31 O32 Mo6 132(2) . 5_575
O30 O32 Mo6 122(2) 5_575 5_575
Mo4 O32 Mo6 92.3(11) . 5_575
Mo2 O32 Mo6 91.7(11) 5_575 5_575
O31 P1 O31 180(2) . 5_575
O31 P1 O30 65.9(18) . .
O31 P1 O30 114.1(18) 5_575 .
O31 P1 O30 114.1(18) . 5_575
O31 P1 O30 65.9(18) 5_575 5_575
O30 P1 O30 180.000(6) . 5_575
O31 P1 O32 112.1(18) . 5_575
O31 P1 O32 67.9(18) 5_575 5_575
O30 P1 O32 69.8(17) . 5_575
O30 P1 O32 110.2(17) 5_575 5_575
O31 P1 O32 67.9(18) . .
O31 P1 O32 112.1(18) 5_575 .
O30 P1 O32 110.2(17) . .
O30 P1 O32 69.8(17) 5_575 .
O32 P1 O32 180(3) 5_575 .
O31 P1 O29 72.6(19) . .
O31 P1 O29 107.4(19) 5_575 .
O30 P1 O29 107.3(18) . .
O30 P1 O29 72.7(18) 5_575 .
O32 P1 O29 74.7(18) 5_575 .
O32 P1 O29 105.3(18) . .
O31 P1 O29 107.4(19) . 5_575
O31 P1 O29 72.6(19) 5_575 5_575
O30 P1 O29 72.7(18) . 5_575
O30 P1 O29 107.3(18) 5_575 5_575
O32 P1 O29 105.3(18) 5_575 5_575
O32 P1 O29 74.7(18) . 5_575
O29 P1 O29 180(2) . 5_575
O19 Mo1 O17 102.5(15) . .
O19 Mo1 O15 102.3(14) . .
O17 Mo1 O15 96.4(11) . .
O19 Mo1 O18 100.2(14) . .
O17 Mo1 O18 155.7(13) . .
O15 Mo1 O18 87.3(10) . .
O19 Mo1 O12 100.5(12) . .
O17 Mo1 O12 86.6(9) . .
O15 Mo1 O12 155.8(13) . .
O18 Mo1 O12 80.7(10) . .
O19 Mo1 O30 160.3(14) . .
O17 Mo1 O30 94.3(13) . .
O15 Mo1 O30 65.1(13) . .
O18 Mo1 O30 65.4(12) . .
O12 Mo1 O30 90.7(11) . .
O19 Mo1 O31 160.0(13) . .
O17 Mo1 O31 66.4(12) . .
O15 Mo1 O31 95.6(13) . .
O18 Mo1 O31 89.3(13) . .
O12 Mo1 O31 63.5(11) . .
O30 Mo1 O31 39.0(11) . .
O24 Mo2 O25 104.5(13) . .
O24 Mo2 O27 102.6(14) . .
O25 Mo2 O27 96.8(12) . .
O24 Mo2 O15 99.6(12) . .
O25 Mo2 O15 87.3(10) . .
O27 Mo2 O15 155.5(14) . .
O24 Mo2 O22 98.7(13) . .
O25 Mo2 O22 155.3(13) . .
O27 Mo2 O22 86.1(10) . .
O15 Mo2 O22 80.5(11) . .
O24 Mo2 O32 158.4(12) . 5_575
O25 Mo2 O32 94.3(12) . 5_575
O27 Mo2 O32 64.1(13) . 5_575
O15 Mo2 O32 91.6(12) . 5_575
O22 Mo2 O32 64.8(12) . 5_575
O24 Mo2 O30 158.2(12) . .
O25 Mo2 O30 65.8(11) . .
O27 Mo2 O30 98.1(13) . .
O15 Mo2 O30 61.6(12) . .
O22 Mo2 O30 89.4(13) . .
O32 Mo2 O30 41.8(11) 5_575 .
O11 Mo3 O13 103.3(15) . .
O11 Mo3 O26 101.2(13) . .
O13 Mo3 O26 94.4(13) . .
O11 Mo3 O23 102.5(14) . .
O13 Mo3 O23 87.7(11) . .
O26 Mo3 O23 155.0(14) . .
O11 Mo3 O17 101.7(13) . .
O13 Mo3 O17 154.3(14) . .
O26 Mo3 O17 86.2(10) . .
O23 Mo3 O17 81.4(11) . .
O11 Mo3 O29 159.1(14) . .
O13 Mo3 O29 62.7(14) . .
O26 Mo3 O29 95.6(13) . .
O23 Mo3 O29 63.3(13) . .
O17 Mo3 O29 91.7(12) . .
O21 Mo4 O12 103.8(12) . .
O21 Mo4 O28 101.4(15) . .
O12 Mo4 O28 95.5(12) . .
O21 Mo4 O26 100.6(13) . .
O12 Mo4 O26 88.5(10) . .
O28 Mo4 O26 156.0(13) . .
O21 Mo4 O27 98.4(13) . 5_575
O12 Mo4 O27 156.8(13) . 5_575
O28 Mo4 O27 86.3(10) . 5_575
O26 Mo4 O27 81.0(11) . 5_575
O21 Mo4 O32 157.7(12) . .
O12 Mo4 O32 96.6(12) . .
O28 Mo4 O32 67.3(13) . .
O26 Mo4 O32 88.7(12) . .
O27 Mo4 O32 62.8(12) 5_575 .
O21 Mo4 O31 161.0(13) . .
O12 Mo4 O31 64.8(12) . .
O28 Mo4 O31 95.1(14) . .
O26 Mo4 O31 65.2(11) . .
O27 Mo4 O31 92.0(13) 5_575 .
O32 Mo4 O31 40.2(11) . .
O14 Mo5 O18 104.4(13) . 5_575
O14 Mo5 O16 103.0(15) . .
O18 Mo5 O16 96.5(13) 5_575 .
O14 Mo5 O13 99.7(14) . .
O18 Mo5 O13 154.2(14) 5_575 .
O16 Mo5 O13 86.6(11) . .
O14 Mo5 O25 101.8(12) . 5_575
O18 Mo5 O25 87.2(10) 5_575 5_575
O16 Mo5 O25 153.1(13) . 5_575
O13 Mo5 O25 79.1(11) . 5_575
O14 Mo5 O29 154.9(12) . .
O18 Mo5 O29 98.4(13) 5_575 .
O16 Mo5 O29 63.7(13) . .
O13 Mo5 O29 60.1(13) . .
O25 Mo5 O29 89.4(12) 5_575 .
O20 Mo6 O22 102.1(13) . .
O20 Mo6 O23 103.4(13) . .
O22 Mo6 O23 96.4(14) . .
O20 Mo6 O16 100.6(13) . .
O22 Mo6 O16 155.8(14) . .
O23 Mo6 O16 86.5(11) . .
O20 Mo6 O28 98.2(12) . 5_575
O22 Mo6 O28 87.8(11) . 5_575
O23 Mo6 O28 156.5(14) . 5_575
O16 Mo6 O28 80.7(12) . 5_575
O20 Mo6 O29 156.7(11) . .
O22 Mo6 O29 98.5(14) . .
O23 Mo6 O29 63.2(13) . .
O16 Mo6 O29 61.3(12) . .
O28 Mo6 O29 93.3(13) 5_575 .
O20 Mo6 O32 156.9(11) . 5_575
O22 Mo6 O32 65.2(12) . 5_575
O23 Mo6 O32 97.3(14) . 5_575
O16 Mo6 O32 90.6(13) . 5_575
O28 Mo6 O32 63.5(11) 5_575 5_575
O29 Mo6 O32 45.2(11) . 5_575
O1 C1 N3 125(3) . 2_554
O1 C1 N1 126(3) . .
N3 C1 N1 109(2) 2_554 .
O6 C2 N3 112(2) . .
O6 C2 N1 108(2) . .
N3 C2 N1 115(2) . .
O6 C2 C2 115.3(14) . 2_554
N3 C2 C2 103(2) . 2_554
N1 C2 C2 103(2) . 2_554
N1 C3 N2 114(2) . .
N1 C3 H3A 108.8 . .
N2 C3 H3A 108.8 . .
N1 C3 H3B 108.8 . .
N2 C3 H3B 108.8 . .
H3A C3 H3B 107.6 . .
N3 C4 N4 112(2) . .
N3 C4 H4A 109.1 . .
N4 C4 H4A 109.1 . .
N3 C4 H4B 109.1 . .
N4 C4 H4B 109.1 . .
H4A C4 H4B 107.8 . .
O2 C5 N5 126(3) . .
O2 C5 N2 126(3) . .
N5 C5 N2 108(3) . .
O2 C5 K1 41.1(14) . .
N5 C5 K1 115.4(18) . .
N2 C5 K1 119.2(17) . .
O7 C6 N2 112(2) . .
O7 C6 N4 110(2) . .
N2 C6 N4 115(2) . .
O7 C6 C7 116(2) . .
N2 C6 C7 103(2) . .
N4 C6 C7 102(2) . .
O8 C7 N5 112(2) . .
O8 C7 N7 110(2) . .
N5 C7 N7 115(2) . .
O8 C7 C6 115(2) . .
N5 C7 C6 102(2) . .
N7 C7 C6 103(2) . .
O4 C8 N4 126(2) . .
O4 C8 N7 125(3) . .
N4 C8 N7 109(2) . .
O4 C8 K1 38.0(15) . 2_554
N4 C8 K1 118.8(17) . 2_554
N7 C8 K1 116.2(18) . 2_554
N5 C9 N6 115(2) . .
N5 C9 H9A 108.5 . .
N6 C9 H9A 108.5 . .
N5 C9 H9B 108.5 . .
N6 C9 H9B 108.5 . .
H9A C9 H9B 107.5 . .
N8 C10 N7 115(2) . .
N8 C10 H10A 108.6 . .
N7 C10 H10A 108.6 . .
N8 C10 H10B 108.6 . .
N7 C10 H10B 108.6 . .
H10A C10 H10B 107.6 . .
O3 C11 N6 127(3) . .
O3 C11 N9 125(3) . .
N6 C11 N9 108(2) . .
O3 C11 K1 38.6(14) . .
N6 C11 K1 114.8(18) . .
N9 C11 K1 121.3(17) . .
O9 C12 N8 109(2) . .
O9 C12 N6 111(2) . .
N8 C12 N6 114(2) . .
O9 C12 C13 116(2) . .
N8 C12 C13 102(2) . .
N6 C12 C13 103(2) . .
O10 C13 N10 111(2) . .
O10 C13 N9 110(2) . .
N10 C13 N9 115(2) . .
O10 C13 C12 115(2) . .
N10 C13 C12 104(2) . .
N9 C13 C12 102(2) . .
O5 C14 N10 126(3) . .
O5 C14 N8 125(3) . .
N10 C14 N8 110(2) . .
O5 C14 K1 37.3(14) . 2_554
N10 C14 K1 117.4(18) . 2_554
N8 C14 K1 117.8(18) . 2_554
N10 C15 N9 113(2) 2_554 .
N10 C15 H15A 108.9 2_554 .
N9 C15 H15A 108.9 . .
N10 C15 H15B 108.9 2_554 .
N9 C15 H15B 108.9 . .
H15A C15 H15B 107.7 . .
C1 N1 C2 112(2) . .
C1 N1 C3 122(2) . .
C2 N1 C3 125(2) . .
C5 N2 C6 113(2) . .
C5 N2 C3 124(2) . .
C6 N2 C3 123(2) . .
C1 N3 C2 113(2) 2_554 .
C1 N3 C4 124(2) 2_554 .
C2 N3 C4 124(2) . .
C8 N4 C4 124(2) . .
C8 N4 C6 113(2) . .
C4 N4 C6 123(2) . .
C5 N5 C7 114(2) . .
C5 N5 C9 124(2) . .
C7 N5 C9 122(2) . .
C11 N6 C12 113(2) . .
C11 N6 C9 122(2) . .
C12 N6 C9 124(2) . .
C8 N7 C7 113(2) . .
C8 N7 C10 123(2) . .
C7 N7 C10 123(2) . .
C14 N8 C12 113(2) . .
C14 N8 C10 123(2) . .
C12 N8 C10 124(2) . .
C11 N9 C15 123(2) . .
C11 N9 C13 113(2) . .
C15 N9 C13 124(2) . .
C14 N10 C13 112(2) . .
C14 N10 C15 123(2) . 2_554
C13 N10 C15 125(2) . 2_554
C1 O1 K1 124.1(18) . .
C5 O2 K1 121.1(18) . .
C11 O3 K1 124.6(18) . .
C8 O4 K1 126(2) . 2_554
C14 O5 K1 126.3(19) . 2_554
C2 O6 H6 109.5 . .
C6 O7 H7 109.5 . .
C7 O8 H8 109.5 . .
C12 O9 H9 109.5 . .
C13 O10 H10 109.5 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
O1W K1 2.26(4) .
O2W K1 3.10(8) 4_544
N11 O34 1.251(6) .
N11 O33 1.292(6) .
N11 O33 1.292(6) 2_554
N11 K1 3.276(6) 2_554
N11 K1 3.276(6) .
O33 K1 2.30(3) 2_554
K1 O33 2.30(3) 2_554
K1 O3 2.58(2) .
K1 O2 2.60(2) .
K1 O5 2.64(2) 2_554
K1 O4 2.68(2) 2_554
K1 O1 2.74(2) .
K1 O2W 3.10(8) 4_554
K1 C5 3.38(3) .
K1 C11 3.41(3) .
K1 C14 3.52(3) 2_554
O11 Mo3 1.64(3) .
O12 Mo4 1.82(2) .
O12 Mo1 1.99(2) .
O13 Mo3 1.80(3) .
O13 Mo5 1.98(3) .
O14 Mo5 1.64(2) .
O15 Mo1 1.82(2) .
O15 Mo2 1.99(2) .
O16 Mo5 1.83(2) .
O16 Mo6 1.97(3) .
O17 Mo1 1.81(2) .
O17 Mo3 1.98(2) .
O18 Mo5 1.82(3) 5_575
O18 Mo1 1.98(2) .
O19 Mo1 1.66(2) .
O20 Mo6 1.65(2) .
O21 Mo4 1.64(2) .
O22 Mo6 1.81(3) .
O22 Mo2 2.00(2) .
O23 Mo6 1.83(3) .
O23 Mo3 1.96(2) .
O24 Mo2 1.66(2) .
O25 Mo2 1.79(2) .
O25 Mo5 1.99(2) 5_575
O26 Mo3 1.85(2) .
O26 Mo4 1.94(2) .
O27 Mo2 1.84(2) .
O27 Mo4 1.97(2) 5_575
O28 Mo4 1.85(2) .
O28 Mo6 1.99(3) 5_575
O29 P1 1.61(4) .
O29 Mo3 2.40(4) .
O29 Mo5 2.43(3) .
O29 Mo6 2.47(4) .
O30 P1 1.52(3) .
O30 O31 1.63(5) .
O30 O32 1.76(5) 5_575
O30 Mo1 2.41(3) .
O30 Mo2 2.49(3) .
O31 P1 1.47(3) .
O31 O32 1.69(5) .
O31 Mo1 2.46(3) .
O31 Mo4 2.49(3) .
O32 P1 1.55(3) .
O32 O30 1.76(5) 5_575
O32 Mo4 2.43(3) .
O32 Mo2 2.44(3) 5_575
O32 Mo6 2.52(3) 5_575
P1 O31 1.47(3) 5_575
P1 O30 1.52(3) 5_575
P1 O32 1.55(3) 5_575
P1 O29 1.61(4) 5_575
Mo2 O32 2.44(3) 5_575
Mo4 O27 1.97(2) 5_575
Mo5 O18 1.82(3) 5_575
Mo5 O25 1.99(2) 5_575
Mo6 O28 1.99(3) 5_575
Mo6 O32 2.52(3) 5_575
C1 O1 1.21(3) .
C1 N3 1.37(3) 2_554
C1 N1 1.37(4) .
C2 O6 1.38(3) .
C2 N3 1.43(3) .
C2 N1 1.45(3) .
C2 C2 1.58(5) 2_554
C3 N1 1.45(3) .
C3 N2 1.46(4) .
C3 H3A 0.9800 .
C3 H3B 0.9800 .
C4 N3 1.45(3) .
C4 N4 1.45(3) .
C4 H4A 0.9800 .
C4 H4B 0.9800 .
C5 O2 1.21(3) .
C5 N5 1.35(4) .
C5 N2 1.37(4) .
C6 O7 1.38(3) .
C6 N2 1.42(4) .
C6 N4 1.47(3) .
C6 C7 1.59(4) .
C7 O8 1.39(3) .
C7 N5 1.43(4) .
C7 N7 1.44(3) .
C8 O4 1.23(3) .
C8 N4 1.35(4) .
C8 N7 1.36(3) .
C8 K1 3.54(3) 2_554
C9 N5 1.45(4) .
C9 N6 1.45(4) .
C9 H9A 0.9800 .
C9 H9B 0.9800 .
C10 N8 1.44(4) .
C10 N7 1.44(4) .
C10 H10A 0.9800 .
C10 H10B 0.9800 .
C11 O3 1.20(3) .
C11 N6 1.37(4) .
C11 N9 1.37(4) .
C12 O9 1.39(3) .
C12 N8 1.44(4) .
C12 N6 1.44(4) .
C12 C13 1.58(4) .
C13 O10 1.37(3) .
C13 N10 1.44(3) .
C13 N9 1.46(4) .
C14 O5 1.23(3) .
C14 N10 1.34(4) .
C14 N8 1.38(4) .
C14 K1 3.52(3) 2_554
C15 N10 1.45(4) 2_554
C15 N9 1.45(4) .
C15 H15A 0.9800 .
C15 H15B 0.9800 .
N3 C1 1.37(3) 2_554
N10 C15 1.45(4) 2_554
O4 K1 2.68(2) 2_554
O5 K1 2.64(2) 2_554
O6 H6 0.8300 .
O7 H7 0.8300 .
O8 H8 0.8300 .
O9 H9 0.8300 .
O10 H10 0.8300 .
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 0.500 0.000 0.000 214 89 ' '
2 0.500 0.000 0.500 214 89 ' '
3 0.095 0.097 0.173 7 7 ' '
4 0.905 0.097 0.327 7 7 ' '
5 0.000 0.500 0.500 214 89 ' '
6 1.000 0.500 1.000 214 89 ' '
7 0.595 0.403 0.673 7 7 ' '
8 0.405 0.403 0.827 7 7 ' '
9 0.595 0.597 0.173 7 7 ' '
10 0.405 0.597 0.327 7 7 ' '
11 0.095 0.903 0.673 7 7 ' '
12 0.905 0.903 0.827 7 7 ' '
